Upload
others
View
6
Download
0
Embed Size (px)
Citation preview
Cite this: RSC Advances, 2013, 3,9365
Molecular and continuum hydrodynamics in graphenenanopores3
Received 6th February 2013,Accepted 19th April 2013
DOI: 10.1039/c3ra40661j
www.rsc.org/advances
M. E. Suk and N. R. Aluru*
An ultrathin graphene membrane is a promising candidate for various applications such as gas separation,
water purification, biosensors, etc. In this study, we investigate water transport mechanisms and
hydrodynamic properties such as water flux, pressure variation, velocity, viscosity, slip length, etc. Due to
the unique water structure, confined in the radial direction and layered in the axial direction of the pore,
water viscosity and slip length increase with a decrease in the pore radius, in contrast to water confined in
a carbon nanotube. As the diameter of the pore increases, the water transport mechanism transitions from
collective diffusion to frictional flow described by the modified Hagen–Poiseuille equation. Graphene
membrane is shown to be ultra-efficient by comparing the permeation coefficient of graphene membrane
to that of a carbon nanotube and an ultrathin silicon membrane. We envision that the study presented
here will help to understand and design various membrane separation processes using graphene
membrane.
1. Introduction
Advances in fabrication, measurement and characterizationhave led to intense research in the area of nanoporousmembranes.1 High performance membranes, that can exhibitsuperior selectivity and high flux, can find numerous applica-tions. For example, efficient water filtration and desalinationcan reduce energy consumption, which can have a positiveeffect on both the water shortage problem2,3 and the growingenergy crisis.4 Nanoporous membranes that are selectivelytransporting ions or delivering biomolecules such as DNA, canlead to further advances in biological research and assist inthe development of lab-on-a-chip devices or biosensors.1,5 Gasseparations, including hydrogen and carbon dioxide separa-tion, using nanoporous membranes can enable advances inclean energy technology.6 These and many other applicationscan benefit from advances in novel and energy efficientnanoporous membranes.
Recently, carbon nanotubes (CNT) have gained significantinterest as nanoporous membranes as they have been shownto be efficient for mass transport due to smooth andhydrophobic surface.7 It was shown that water flow rate
through a CNT membrane is three to four orders of magnitudehigher compared to that from the no-slip Hagen–Poiseuille’s(HP) equation.8,9 Molecular dynamics (MD) simulations haveshown a large amount of liquid slip at the nanotube surface,representing low frictional resistance.10,11 Recently, silicon-based membranes were fabricated with a membrane thicknessof 15 nm12,13 to increase the efficiency by reducing themembrane length. Even though silicon-based membranes didnot show the dominant liquid slip at the surface13 due to thehydrophilic nature of the surface, flow rate through thesemembranes were higher compared to that through thickermembranes made of a silica–surfactant nanocomposite12 orCNT.13
Owing to its ultra-small thickness, nanoporous graphenemembranes are promising candidates for various applications.Since the graphene membrane is only a single-atom thick, itcan be considered as the thinnest membrane possible.Nanopores of various diameters can be realized in grapheneby irradiation with an electron beam.14 Nanopores in grapheneare known to be stable over time despite the extreme thinnessof graphene.15 Due to its robustness and potential, nanopor-ous graphene has been suggested for DNA sequencing.15–17 Inaddition, various applications such as ion and gas separationhave also been proposed.18,19
Understanding water transport mechanisms and hydro-dynamic properties in membranes is essential to characterizeand design membranes for various applications mentionedabove. In nanopores, water transport mechanisms can differfrom the continuum hydrodynamics description and waterproperties under confinement can be different from the bulkvalues. Numerous theoretical and experimental studies have
Department of Mechanical Science and Engineering, Beckman Institute for Advanced
Science and Technology, University of Illinois at Urbana-Champaign, Urbana, Illinois
61801, USA. E-mail: [email protected]
3 Electronic supplementary information (ESI) available: Water velocity profile inthe axial direction. No-slip hydrodynamics by Dagan et al. Calculation ofviscosity and slip length using NEMD and Green-Kubo relation. Definition ofpore radius and length. Calculation of diffusion coefficient and collectivediffusion coefficient. Effect of thermal motion of graphene membrane. See DOI:10.1039/c3ra40661j
RSC Advances
PAPER
This journal is � The Royal Society of Chemistry 2013 RSC Adv., 2013, 3, 9365–9372 | 9365
been performed to understand structure, dynamics andtransport of water confined in CNTs8–11 and in grapheneslabs.20,21 However, very little is known regarding watertransport through graphene nanopores despite their promis-ing characteristics. Hydrodynamics and frictional losses canbe quite different in graphene membranes compared tothicker membranes and these need to be understood in greatdetail to realize the full potential of graphene nanopores. Inthis paper, we perform detailed studies to understand watertransport mechanisms and hydrodynamic properties of waterin various diameter graphene nanopores.
2. Methods
We performed molecular dynamics (MD) simulations of waterflow through graphene nanopores. Fig. 1 shows the simulationsetup and water-filled graphene nanopores of various dia-meters. Pore radii we considered in this work are 0.283 nm,0.424 nm, 0.704 nm, 0.933 nm, 1.169 nm, 1.511 nm and 1.888nm. Pore radius is determined by measuring the distance fromthe pore axis to the location where the water density droppedto below 2% of bulk value (see ESI3 for determination of thepore radius). Corresponding center-to-center radii calculatedby averaging the distance from the pore axis to the center ofthe carbon atoms in the pore edge are 0.424 nm, 0.526 nm,0.911 nm, 1.136 nm, 1.374 nm, 1.687 nm and 2.083 nm.Graphene pores are generated by removing atoms whosecoordinates satisfy the condition (x 2 Cx)2 + (y 2 Cy)2 , R2
where Cx and Cy are the x and y coordinates of the pore center,respectively. Pores are not passivated to remove any effect frompassivating atoms such as charges and interaction energies.
The carbon atoms of the graphene membrane weremodeled as Lennard-Jones spheres with the parameters s =0.339 nm and e = 0.2897 kJ mol21.22 Water molecules weremodeled using the simple point charge-extended (SPC/E) watermodel.23 Both x and y dimensions of the graphene membrane(see Fig. 1) range from about 4 nm to 8 nm in lengthdepending on the pore radius to keep the porosity (pore area/total membrane area) constant. The z dimension of the totalsystem is approximately 12 nm in length. The graphenemembrane is centered separating the two water baths. Thetotal number of water molecules varied from 6479 to 24 046,depending on the system size. Periodic boundary conditionwas applied in all the three-directions. Nose-Hoover thermo-stat was used to maintain the temperature at 300 K with a timeconstant of 0.1 ps. Graphene membranes were kept rigidduring the simulation by fixing carbon atoms to their latticepositions. Thermal motion of graphene had negligible effecton results (see ESI3). SETTLE algorithm was used to constrainthe angle and bond length of SPC/E water. It is reported thatflexible water models produce similar water dynamics ingraphene nanopores.24
Equation of motion was integrated with a 1 fs time step.The simulation box size in the z direction was adjusted tomaintain the system pressure at 1 bar for 1 ns and then an
NVT ensemble was run for 1 ns to attain an initial equilibriumconfiguration. For pressure-driven flow simulation, an externalpressure drop was applied using the method proposed by Zhuet al.25 for an additional 10y20 ns after the equilibration run.Pressure drop was created by applying external forces on theoxygen atoms of the water molecules in the Dz = 1 nm slabregion at the end of system.26 Applied force on an individualwater molecule is given by, f = DPA/n where DP is the desiredpressure drop, A is the area of the membrane and n is the totalnumber of water molecules on which the external force isapplied.25 For the Green-Kubo (GK) calculations, equilibriumMD simulations were run for 5 ns with data sampling every 20fs. For the calculation of the diffusion coefficient and thecollective diffusion coefficient, equilibrium simulation wasrun for 10 ns with data sampling every 500 fs. All thesimulations were performed using Gromacs.27
3. Results and discussion
3.1 Pressure driven flow
A total pressure drop, DPtotal, varying from 10 MPa to 300 MPais applied across the graphene membrane. Water flux ismeasured by counting the number of water moleculestransported through the pore during the course of thesimulation time and is shown in Fig. 2(b). A linear relationbetween water flux and the total pressure drop is observed asshown in Fig. 2(b).
We found that the variation of the local pressure normalizedby the applied total pressure drop is nearly identical (seeFig. 2(a)) for various pressure drops. This indicates that theentrance and exit pressure loss is proportional to the appliedtotal pressure drop. Thus, water flux is also proportional to theapplied total pressure drop as shown in Fig. 2(b). Such flowbehavior can be explained by the low Reynolds numbercreeping flow predicting a linear relation between flow rateand the total pressure drop.28–30 Although a high pressure
Fig. 1 Visualization of water molecules permeating through graphene nano-pores of various radii. Graphene membranes are shown in blue. Watermolecules are described by red (oxygen) and white (hydrogen) spheres. Poreradii are R = 0.424 nm (left top) R = 0.933 nm (left bottom) and R = 1.51 nm(right).
9366 | RSC Adv., 2013, 3, 9365–9372 This journal is � The Royal Society of Chemistry 2013
Paper RSC Advances
drop is applied, the Reynolds number is of the order of0.01y0.1 in the present study. Since viscous term is dominantin low Reynolds number flow, Hagen–Poiseuille(HP)’s flow isproposed and corrected in the next section to predict thepermeation coefficient of graphene nanopores. The deviationsof water properties in graphene nanopores from the bulkproperties are also investigated.
3.2 Corrected Hagen–Poiseuille’s equation and hydrodynamicmembrane length
The flow domain is symmetric and our results indicate thatdu/dz = 0 at the pore center (z = zc) where u is the velocity in theaxial direction (see ESI3). Under the assumption, du/dz = 0, HPequation can be derived from the mass and momentumconservation equations. Using the HP equation modified bythe slip boundary condition, fluid velocity in the radialdirection is given by
u(r)~ {1
4mr2z
R2
4mz
R
2md
� �dP
dz(1)
where m is the viscosity, R is the pore radius and d is the sliplength satisfying d = u(R)(du/dr)r=R (r = 0 is pore center).Although the graphene nanopore region is very thin, anapproximately linear pressure drop (see inset of Fig. 2(a)) and a
near uniform velocity in the axial direction (see inset of Fig. S1in ESI3) indicate that the HP equation can be used to obtaingood insights into transport through the nanopore. dP/dz isusually obtained by DPp/Lp, by taking into account entranceand exit pressure losses, where Lp is the pore length depictedin Fig. 2(a), and DPp is the pressure drop across the porelength Lp. DPp = DPtotal 2 DPloss, where DPloss is the pressureloss at the entrance and exit. To simplify calculation of dP/dz,where the total applied pressure drop, DPtotal, is used, wedefine a hydrodynamic membrane length as, Lh = DPtotal/(dP/dz). Then, dP/dz can be computed as DPtotal/Lh. Lh isgraphically depicted in Fig. 2(a). We note that Lh isindependent of the applied pressure drop or fluid velocity,and it effectively takes into account the entrance and exitpressure losses. Lh is obtained using a linear fit to the variationof P(z)/DPtotal with the axial direction (z) in the pore region (seeinset of Fig. 2(a)). Averaged fit is superimposed in the inset ofFig. 2(a) with a solid line.
Since Lh is a geometrical variable, it depends on the poreradius. We repeated the calculation of hydrodynamic length Lh
for various pore radii and this is plotted in Fig. 2(c). Lh
increases linearly with the pore radius and it is given by theempirical relation
Fig. 2 (a) Pressure distribution normalized by the total applied pressure drop along the flow direction. The three different symbols indicate total applied pressuredrops of 100 MPa, 200 MPa and 300 MPa. Normalized pressure distributions are close to each other and are represented by a solid line. Graphene pore length (Lp)and hydrodynamic membrane length (Lh) are graphically depicted. Lp = 0.54 nm and Lh = 1.25 nm for pore radius of 1.169 nm. (Inset) Closer view of linear pressuredistribution inside the pore. (b) Water flux through various radii graphene nanopores. Water flux is linear with applied pressure drop. (c) Variation of thehydrodynamic membrane length with graphene pore radius. Hydrodynamic membrane length increases linearly with the pore radius. Solid line is a linear fit of thedata.
This journal is � The Royal Society of Chemistry 2013 RSC Adv., 2013, 3, 9365–9372 | 9367
RSC Advances Paper
Lh = 0.27R + 0.95 (2)
The solid line in Fig. 2(c) represents the relation given ineqn (2). For low Reynolds number hydrodynamics, the theorydeveloped by Dagan et al.28 can be used to derive an expressionfor Lh and we note that Lh depends linearly on the pore radiusin Dagan et al. theory as well (see ESI3) However, Dagan’sequation is developed under the assumption of no-slipboundary condition where the fluid velocity is zero at thewall. Thus, Dagan’s equation is not directly applicable forwater transport through graphene due to the slip boundarycondition.
By introducing Lh, eqn (1) can be modified as,
u(r)~ {1
4mr2z
R2
4mz
R
2md
� �DPtotal
Lh(3)
The accuracy of eqn (3)will depend on water properties suchas viscosity m and slip length d and geometrical variables suchas the pore radius R and the hydrodynamic membrane lengthLh.
Water transport properties such as viscosity m and sliplength d can be obtained using non equilibrium MD (NEMD)or equilibrium MD (EMD) simulations. In an NEMD simula-tion, liquid flow is driven by an external field such as gravity,pressure gradient or shear stress and liquid properties can becalculated by comparing the velocity profile to standardmodels such as Poiseuille’s flow or Couette flow. On the otherhand, in an EMD simulation, liquid properties can beobtained by applying Green-Kubo (GK) relations, which areexpressed as auto-correlation functions of variables fluctuatingat equilibrium. In certain cases, these methods can result ininaccurate liquid properties (see ESI3 for more discussion). Toobtain accurate water properties, in this work, we investigateboth NEMD and EMD simulations and found good agreementas shown in Fig. 3(a) and Fig. 3(b). Detailed calculation
procedure on NEMD and EMD method can be found in theESI.3 In addition, calculation of m and d can be sensitive to thesmall change in pore radius R and pore length Lp. Thus, aproper and consistent definition of the pore radius and lengthis necessary. We defined R and Lp based on water density byfinding location where water density dropped below 2%. Morediscussion on this can be found in the ESI.3
Velocity profile u(r) obtained by substituting m and d
calculated from the GK relations into eqn (3) is compared tothe NEMD pressure-driven flow simulation in Fig. 3(c). Sincethe agreement is good, we can conclude that water flowthrough the graphene nanopore can be predicted by thecorrected HP equation.
In the next section, the variation of viscosity and slip lengthwith the pore radius is investigated.
3.3 Variation of viscosity and slip length with radius of thegraphene nanopore
We investigated the variation of viscosity and slip length withthe pore radius and these are shown in Fig. 4(a) and 4(b),respectively. These are obtained using GK relations. Bothviscosity and slip length monotonically decrease with theincrease in the pore radius. At the limit of infinite pore radius,viscosity should approach the bulk viscosity, mbulk = 0.00085Pa?s31 and the corresponding slip length is dRA‘ = 0.205 nm.dRA‘ is calculated from friction coefficient of a flat graphenenano slit whose separation width is 1.169 nm. This is tocapture the case of R A ‘. Since Cieplak et al.32 reported thatthe slip length is independent of the separation width of thechannel, it can be concluded that the degree of curvaturemainly contributes to the variation of the friction coefficientwith the radius. Variation of m and d with the pore radius aregiven by the empirical relations,
m(R) = C1/R + 0.00085 Pa s (4)and
d(R) = C2/R + 0.205 nm (5)
Fig. 3 (a) Viscosity and (b) slip length calculated using NEMD simulations and Green-Kubo (GK) relation. (c) Comparison of velocity profiles from NEMD simulationsand corrected HP equation with water properties obtained from the GK relation. In NEMD simulation, velocity profile is calculated by averaging the center-of-massvelocities of individual water molecules located in the cylindrical region centered about the pore axis and the length of cylinder is equal to the carbon diameter. Eachline and squared symbol profile represents a different pressure drop, DP = 10 MPa, 50 MPa, 100 MPa, 200 MPa and 300 MPa. Data is obtained for R = 1.169 nm pore.
9368 | RSC Adv., 2013, 3, 9365–9372 This journal is � The Royal Society of Chemistry 2013
Paper RSC Advances
where R is pore radius in nm, and C1 and C2 are the unknowncoefficients. By using a least-squares method, C1 and C2 aredetermined to be 0.000847 Pa s nm and 0.1517 nm2,respectively. These relations are plotted in Fig. 4(a) and (b)as a solid line.
Slip length and viscosity of water confined in a graphenenanopore are different from those in a CNT. Slip length ofwater in a graphene nanopore is significantly smallercompared to that in a CNT. At the water/CNT interface, sliplength ranges from several hundreds to tens of thousands ofnanometers.8,9 The viscosity of water confined in a graphenenanopore is higher than that of water confined in a similardiameter CNT.11,33,34 Variation of water viscosity and sliplength with the pore radius in the case of graphene is alsodifferent from that of in the infinite CNT. Slip length of waterconfined in the CNT decreases with the increase in poreradius11 as d y 1/r3, while the slip length of water movingoutside the CNT increased with the CNT radius.35 Viscosity ofwater confined in the CNT increases with the increase in poreradius until it approaches the bulk viscosity.11,33,34 Theincrease in viscosity with the decrease in radius in graphenenanopore is related to the water structure, which is discussedin the next section. Due to the statistical inaccuracy, waterviscosity and slip length are not measured for R = 0.283 nmand R = 0.424 nm graphene nanopores.
3.4 Density and diffusion coefficient
Water structure along the axial direction in a graphenenanopore is unique and different from that in the interior ofthe CNT. Layered water structure, described by densityoscillations in the radial direction, at the surface of the CNTwas reported by various authors.10,33,36 In the case of graphenenanopore, similar water layering in the radial direction isobserved. However, more importantly, the water molecules arealso layered in the flow/axial direction (z-direction) as shownin Fig. 5(a) and 5(b). Fig. 5(a) and 5(b) indicate that the degreeof density fluctuation increases as the radius of the graphenenanopore decreases. This is due to the increasing influence ofgraphene atoms on the water molecules. As the pore radiusdecreases, an increasing fraction of the water molecules arewithin a distance where the van der Waals interaction betweenthe graphene atoms and the water molecules is significant.
To quantify the water layering effect, we defined the waterlayering factor as WL = (rmax 2 rmin)/rbulk where rmax and rmin
are the maximum and minimum density near the surface.Water layering factor, WL, decreases and approaches zero asthe pore radius increases. We show that viscosity is related tothe water layering effect by noting that viscosity increaseslinearly with the layering factor, WL. This is shown in Fig. 5(c).Using linear extrapolation, we also note in Fig. 5(c) that waterviscosity approaches the bulk viscosity as WL approaches zero.One plausible explanation for the increase in water viscositywith the increase in water layering factor is due to the lowdiffusion of water in the axial direction due to the layeredstructure. It should be noted that water confined in theCNT10,11 or in a nano slab configuration37,38 does notexperience the water layering effect in the flow direction asin the case of the graphene nanopore. Thus, the magnitude ofviscosity or the variation of viscosity with pore radius ingraphene is not consistent with studies on other nanopores.
We calculated the diffusion coefficient in the axial directionto understand the effect of the layered water structure on thewater movement. As shown in Fig. 5(d), diffusion coefficient inthe graphene nanopore is lower than the bulk diffusioncoefficient,39 Dz = 2.69 6 1029 m2 s21. Furthermore, diffusioncoefficient decreases with the decrease in the pore radius. Thisindicates that diffusion coefficient decreases as the effect ofwater layering in the axial direction increases. Water immo-bilization at a critical pore radius, such as the ice-like structurein CNT,39 is not observed. Water diffusion coefficient for R =0.283 nm pore is comparable to that for the R = 0.424 nm pore.In the R = 0.283 nm case, single file water molecules7,26 areobserved. In this case, water molecules are highly correlatedand diffusion coefficient does not necessarily follow the trendobserved for larger pores. Once the variation of the waterproperties with pore radii are obtained, we calculate thepermeation coefficients of graphene nanopores of variousradii using the corrected HP equation. These results arecompared to the results from pressure driven flow simulationand other experimental data in the following section.
3.5 Permeability of graphene nanopore
Permeation coefficient is defined as pQ = Q/DP, where Q is thevolumetric flow rate and DP is the applied pressure drop. A
Fig. 4 (a) Viscosity and (b) slip length obtained using GK relations. Solid lines areempirical fits given by eqn (4) and eqn (5). Dashed lines indicate viscosity andslip length when the radius of the pore approaches infinity.
This journal is � The Royal Society of Chemistry 2013 RSC Adv., 2013, 3, 9365–9372 | 9369
RSC Advances Paper
higher pQ indicates a more energy-efficient membrane thatdelivers more water for a given pressure drop. pQ can bedirectly determined from the NEMD pressure-driven flowsimulation by a linear fitting of Q (or water flux) vs. DP relation(see Fig. 2(b)). The permeation coefficient corresponding tographene nanopores of various diameters is shown in Fig. 6(a).
Permeation coefficient can also be theoretically predictedfrom the corrected HP relation. By integrating u(r) given by eqn(3), Q can be determined as
Q~p(R4z4R3d)
8m
DP
Lh(6)
Thus,
pQ(R)~p(R4z4R3d)
8m
1
Lh(7)
By substituting the empirical relations for Lh(R), m(R) andd(R) (eqn (2), (4) and (5)) obtained in this study, we calculatedpQ(R). This is compared to the permeation coefficient obtainedfrom the NEMD simulation in Fig. 6(a). They are in good
agreement when the graphene pore radius is larger than 0.484nm. pQ calculated from no-slip hydrodynamics is also shownin Fig. 6(a). No-slip hydrodynamics at low Reynolds number isderived by Dagan et al.28 for flow through a circular pore. Wesubstituted a graphene pore length of, Lp = 0.5354 nm intoDagan’s equation,
pQ(R)~pR4
m(3pRz8Lp)(8)
Hydrodynamics through ultrathin hydrophilic membranes,such as porous nanocrystalline silicon (Pnc-si) membranes,have been shown to be in good agreement with Dagan’sequation.13 Enhancement of volumetric flow rate over no-sliphydrodynamics (eqn (8)) approximately ranges from a factor ofthree to five for R = 0.5 nmy2 nm. This enhancement over no-slip hydrodynamics is due to the slip at the surfacerepresenting advantages of hydrophobic surface of graphenepore.
Additionally, we also estimated the permeation coefficientusing the collective diffusion theory40 (see ESI3 for details).Collective diffusion theory assumes that water molecules are
Fig. 5 Water density in the axial direction for (a) radius varying from R = 0.704 nm to R = 1.89 nm and (b) R = 0.283 nm, R = 0.424 nm. z is the axial direction and thegraphene membrane is located at z = 6 nm. (c) Relation between water viscosity and water layering factor. A linear fit is shown by the solid line. (d) Variation of theaxial diffusion coefficient with pore radius.
9370 | RSC Adv., 2013, 3, 9365–9372 This journal is � The Royal Society of Chemistry 2013
Paper RSC Advances
highly correlated and collectively diffuse through the pore by achemical potential gradient. In graphene nanopores, when theradius is smaller than 0.484 nm, the collective diffusion theorygives better approximation compared to the corrected HPrelation (see inset of Fig. 6(a)). In such small nanopores,single-file water molecules7,26 are observed and water–watercorrelation is an important factor for water transport.However, corrected HP relation gives better agreementcompared to the collective diffusion theory as the pore radiusincreases. This indicates that the water transport mechanismtransitions from collective diffusion to frictional flowdescribed by the corrected HP relation. Since the correctedHP equation represents the water permeability of graphenenanopores reasonably well, we compare these results to theexperimental data of CNT and ultrathin silicon membrane inthe next section.
3.6 Comparison of permeability of graphene to CNT andsilicon membranes
Assuming that the expressions presented above for thepermeation coefficient of graphene nanopores are also validwhen the pore radius is larger than 2 nm, we compare thepermeability of graphene membranes to the reported valueson CNT-based membranes8,9,41,42 and ultrathin silicon-basedmembranes.13 Various experimental data are compared inFig. 6(b). The CNT membranes are fabricated with lengthsranging from micrometers to millimeters. Silicon-basedmembranes are fabricated as thin as 15 nm.
Water permeability of the graphene membrane is eithercomparable or higher than that of a CNT, depending on poreradius or length. Due to the large variation in experimentaldata of the CNT for R = 0.83 nm and R = 3.5 nm, it is unclearwhether permeability of graphene is higher than that of theCNT. For R = 1.5 nm and R = 5 nm, CNT length is relativelylong and permeability of the graphene membrane is eight-foldand five-fold higher compared to that of the CNT, respectively.We also compared the permeability of the graphene mem-brane to that of the nanometer-thin Pnc-si membranes13 inFig. 6(b). Pnc-si membranes also have high permeabilitycompared to the commercial ultrafiltration membranes orother types of membranes13 since the nanometer-thin mem-brane length reduces frictional losses. Permeability of thegraphene membrane is approximately four to six-fold highercompared to that of the Pnc-si membrane. Hydrophobicnature of the graphene surface as well as shorter membranelength contributes to the enhanced permeability of thegraphene membrane over the hydrophilic Pnc-si mem-branes.13
4. Conclusions
Hydrodynamics through graphene nanopores can be differentfrom nanopores in thicker or longer membranes. Due to thenanometer dimension of the pore, Reynolds number forpressure-driven water flow through graphene nanopores isvery small and a linear relation between flow rate and appliedpressure drop is observed. Hydrodynamic membrane length isintroduced to effectively capture entrance and exit pressurelosses. Hydrodynamic membrane length is independent of theapplied pressure gradient or fluid velocity, but varies linearlywith the pore radius. Water viscosity and slip length decreasewith the increase in pore radius due to the water layering effectin the flow direction. Velocity profile and permeationcoefficient obtained with the corrected HP equation are foundto be in good agreement with molecular simulations. For thesmall radius pore, where water–water correlation is important,collective diffusion mechanism predicts permeability ofgraphene quite well. Depending on the pore radius or length,permeability of the graphene nanopore can be either compar-able or higher than that of a micrometer-thick CNT mem-brane. In addition, the permeation coefficient of the graphenenanopore is four to six-fold higher compared to that ofnanometer-thick silicon membranes, suggesting that the
Fig. 6 (a) Permeation coefficients of graphene membranes from NEMDsimulations are compared to the theoretical predictions by collective diffusion,40
corrected HP equation (this work) and no-slip hydrodynamics.28 Corrected HPrelation describes permeation coefficient very well for R > 0.5 nm. (b)Theoretically predicted permeation coefficient of graphene membranes bycorrected HP relation is compared to the experimental data of CNTmembranes8,9,41,42 and silicon membranes.13 Some of experimental datareported the permeability based on the membrane area.9,13,42 i.e., pQ = Qtotal/(DP?Am) where Qtotal is the total water flow rate through the membrane and Am
is the membrane area. For direct comparison, these experimental data areconverted to pQ as defined in our study (volumetric water flow per pore/totalapplied pressure).
This journal is � The Royal Society of Chemistry 2013 RSC Adv., 2013, 3, 9365–9372 | 9371
RSC Advances Paper
graphene membrane is a promising candidate for variousapplications.
Acknowledgements
This research is supported by NSF under grants 0852657 and0915718.
References
1 C. Dekker, Nat. Nanotechnol., 2007, 2, 209–215.2 M. A. Shannon, P. W. Bohn, M. Elimelech, J. G. Georgiadis,
B. J. Marinas and A. M. Mayes, Nature, 2008, 452, 301–310.3 T. Hillie and M. Hlophe, Nat. Nanotechnol., 2007, 2,
663–664.4 N. Armaroli and V. Balzani, Angew. Chem., Int. Ed., 2007, 46,
52.5 B. M. Venkatesan and R. Bashir, Nat. Nanotechnol., 2011, 6,
615–624.6 N. W. Ockwig and T. M. Nenoff, Chem. Rev., 2007, 107,
4078–4110.7 G. Hummer, J. C. Rasaiah and J. P. Noworyta, Nature, 2001,
414, 188–190.8 J. K. Holt, H. G. Park, Y. Wang, M. Stadermann, A.
B. Artyukhin, C. P. Grigoropoulos, A. Noy and O. Bakajin,Science, 2006, 312, 1034.
9 M. Majumder, N. Chopra, R. Andrews and B. J. Hinds,Nature, 2005, 438, 44.
10 S. Joseph and N. R. Aluru, Nano Lett., 2008, 8, 452–458.11 J. A. Thomas and A. J. H. McGaughey, Nano Lett., 2008, 8,
2788–2793.12 C. C. Striemer, T. R. Gaborski, J. L. McGrath and P.
M. Fauchet, Nature, 2007, 445, 749–753.13 T. R. Gaborski, J. L. Snyder, C. C. Striemer, D. Z. Fang,
M. Hoffman, P. M. Fauchet and J. L. McGrath, ACS Nano,2010, 4, 6973–6981.
14 M. D. Fischbein and M. Drndi, Appl. Phys. Lett., 2008, 93,113107.
15 C. A. Merchant, K. Healy, M. Wanunu, V. Ray, N. Peterman,J. Bartel, M. D. Fischbein, K. Venta, L. U. O. Zhengtang andA. T. Charlie Johnson, Nano Lett., 2010, 10, 2915–2921.
16 G. F. Schneider, S. W. Kowalczyk, V. E. Calado,G. Pandraud, H. W. Zandbergen, L. M. K. Vandersypenand C. Dekker, Nano Lett., 2010, 10, 3163–3167.
17 S. Garaj, W. Hubbard, A. Reina, J. Kong, D. Branton and J.A. Golovchenko, Nature, 2010, 467, 190–193.
18 K. Sint, B. Wang and P. Kral, J. Am. Chem. Soc., 2008, 130,16448–16449.
19 D. E. Jiang, V. R. Cooper and D. A. I. Sheng, Nano Lett.,2009, 9, 4019–4024.
20 V. P. Sokhan, D. Nicholson and N. Quirke, J. Chem. Phys.,2001, 115, 3878–3887.
21 G. Cicero, J. C. Grossman, E. Schwegler, F. Gygi andG. Galli, J. Am. Chem. Soc., 2008, 130, 1871–1878.
22 G. Chen, Y. Guo, N. Karasawa and W. A. Goddard III, Phys.Rev. B: Condens. Matter, 1993, 48, 13959.
23 H. J. C. Berendsen, J. R. Grigera and T. P. Straatsma, J. Phys.Chem., 1987, 91, 6269–6271.
24 D. Cohen-Tanugi and J. C. Grossman, Nano Lett., 2012, 12,3602–3608.
25 F. Zhu, E. Tajkhorshid and K. Schulten, Biophys. J., 2002,83, 154–160.
26 M. E. Suk and N. R. Aluru, J. Phys. Chem. Lett., 2010, 1,1590–1594.
27 B. Hess, C. Kutzner, D. van der Spoel and E. Lindahl, J.Chem. Theory Comput., 2008, 4, 435–447.
28 Z. Dagan, S. Weinbaum and R. Pfeffer, J. Fluid Mech., 1982,115, 505–523.
29 R. A. Sampson, Philos. Trans. R. Soc. London, Ser. A, 1891,182, 449–518.
30 J. Happel and H. Brenner, Low Reynolds NumberHydrodynamics: With Special Applications To ParticulateMedia, Kluwer Academic, Hingham, 1991.
31 R. C. Weast, CRC Handbook of Chemistry and Physics, CRCPress, Boca Raton, 1986.
32 M. Cieplak, J. Koplik and J. R. Banavar, Phys. Rev. Lett.,2001, 86, 803–806.
33 J. S. Babu and S. P. Sathian, J. Chem. Phys., 2011, 134, 4509.34 H. Zhang, H. Ye, Y. Zheng and Z. Zhang, Microfluid.
Nanofluid., 2011, 10, 403–414.35 J. H. Walther, T. Werder, R. L. Jaffe and P. Koumoutsakos,
Phys. Rev. E: Stat., Nonlinear, Soft Matter Phys., 2004, 69,062201.
36 X. Chen, G. Cao, A. Han, V. K. Punyamurtula, L. Liu, P.J. Culligan, T. Kim and Y. Qiao, Nano Lett., 2008, 8,2988–2992.
37 T.-D. Li, J. Gao, R. Szoszkiewicz, U. Landman and E. Riedo,Phys. Rev. B: Condens. Matter Mater. Phys., 2007, 75, 115415.
38 U. Raviv, S. Giasson, J. Frey and J. Klein, J. Phys.: Condens.Matter, 2002, 14, 9275.
39 R. J. Mashl, S. Joseph, N. R. Aluru and E. Jakobsson, NanoLett., 2003, 3, 589–592.
40 F. Zhu, E. Tajkhorshid and K. Schulten, Phys. Rev. Lett.,2004, 93, 224501.
41 F. Du, L. Qu, Z. Xia, L. Feng and L. Dai, Langmuir, 2011, 27,8437–8443.
42 M. Yu, H. H. Funke, J. L. Falconer and R. D. Noble, NanoLett., 2008, 9, 225–229.
9372 | RSC Adv., 2013, 3, 9365–9372 This journal is � The Royal Society of Chemistry 2013
Paper RSC Advances